widely used in the building industry for waterproofing flat roofs and tanking underground. Mastic asphalt is heated to a temperature of and is spread in layers to form an impervious barrier about thick. Bitumen emulsion Bitumen emulsions are colloidal mixtures of bitumen and water. Due to the different surface tensions of the two liquids, stable emulsions cannot be created simply by mixing. Therefore, various emulsifiers and stabilizers are added. Emulsifiers are amphiphilic molecules that differ in the charge of their polar head group. They reduce the surface tension of the emulsion and thus prevent bitumen particles from fusing. The emulsifier charge defines the type of emulsion: anionic (negatively charged) and cationic (positively charged). The concentration of an emulsifier is a critical parameter affecting the size of the bitumen particles - higher concentrations lead to smaller bitumen particles. Thus, emulsifiers have a great impact on the stability, viscosity, breaking strength, and adhesion of the bitumen emulsion. The size of bitumen particles is usually between 0.1 and 50 µm with a main fraction between 1 µm and 10 µm. Laser diffraction techniques can be used to determine the particle size distribution quickly and easily. Cationic emulsifiers primarily include long-chain amines such as imidazolines, amido-amines, and diamines, which acquire a positive charge when an acid is added. Anionic emulsifiers are often fatty acids extracted from lignin, tall oil, or tree resin saponified with bases such as NaOH, which creates a negative charge. During the storage of bitumen emulsions, bitumen particles sediment, agglomerate (flocculation), or fuse (coagulation), which leads to a certain instability of the bitumen emulsion. How fast this process occurs depends on the formulation of the bitumen emulsion but also storage conditions such as temperature and humidity. When emulsified bitumen gets into contact with aggregates, emulsifiers lose their effectiveness, the emulsion breaks down, and an adhering bitumen film is formed referred to as 'breaking'. Bitumen particles almost instantly create a continuous bitumen film by coagulating and separating from water which evaporates. Not each asphalt emulsion reacts as fast as the other when it gets into contact with aggregates. That enables a classification into Rapid-setting (R), Slow-setting (SS), and Medium-setting (MS) emulsions, but also an individual, application-specific optimization of the formulation and a wide field of application (1). For example, Slow-breaking emulsions ensure a longer processing time which is particularly advantageous for fine aggregates (1). Adhesion problems are reported for anionic emulsions in